Water vapour sorption properties of a family of square lattice topology porous coordination networks.
Shabangu, Samuel M.; Eaby, Alan C.; Croitor, Lilia; Bezrukov, Andrey A.; Zaworotko, Michael J.; CrystEngComm 27 (2025) 5669–5675; doi:10.1039/d5ce00385g

data_7250705
_publ_section_title
;
 Water vapour sorption properties of a family of square lattice topology
 porous coordination networks.
;
_journal_issue                   34
_journal_name_full               CrystEngComm
_journal_page_first              5669
_journal_page_last               5675
_journal_paper_doi               10.1039/d5ce00385g
_journal_volume                  27
_journal_year                    2025
_chemical_formula_sum            'C14 H18 N2 O8 Zn'
_chemical_formula_weight         407.67
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2024-10-11 deposited with the CCDC.	2025-07-23 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 112.118(5)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   19.654(3)
_cell_length_b                   11.4262(14)
_cell_length_c                   7.9610(9)
_cell_measurement_reflns_used    1437
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      17.28
_cell_measurement_theta_min      3.10
_cell_volume                     1656.2(4)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      150(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.2056
_diffrn_reflns_av_unetI/netI     0.1292
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            10772
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        24.982
_diffrn_reflns_theta_max         24.982
_diffrn_reflns_theta_min         3.120
_exptl_absorpt_coefficient_mu    1.529
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.635
_exptl_crystal_description       needle
_exptl_crystal_F_000             840
_exptl_crystal_size_max          0.209
_exptl_crystal_size_mid          0.071
_exptl_crystal_size_min          0.042
_refine_diff_density_max         1.337
_refine_diff_density_min         -0.715
_refine_diff_density_rms         0.125
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.022
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     176
_refine_ls_number_reflns         1465
_refine_ls_number_restraints     7
_refine_ls_restrained_S_all      1.020
_refine_ls_R_factor_all          0.1457
_refine_ls_R_factor_gt           0.0722
_refine_ls_shift/su_max          0.011
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0788P)^2^+2.2844P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1450
_refine_ls_wR_factor_ref         0.1664
_reflns_Friedel_coverage         0.000
_reflns_number_gt                878
_reflns_number_total             1465
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d5ce00385g2.cif
_cod_data_source_block           Zn-alpha1
_cod_depositor_comments
'Adding full bibliography for 7250704--7250705.cif.'
_cod_original_cell_volume        1656.3(4)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               7250705
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.741
_shelx_estimated_absorpt_t_max   0.939
_shelx_res_checksum              793